Phase Transition and Negative Thermal Expansion in Guanidinium Magnesium-Hypophosphite Hybrid Perovskite
Gao, Hong-Qiang; Wei, Wen-Juan; Tan, Yu-Hui; Tang, Yun-Zhi; Chemistry of Materials  (2020) –; doi:10.1021/acs.chemmater.0c01654

data_4003654
_publ_section_title
;
 Phase Transition and Negative Thermal Expansion in Guanidinium
 Magnesium-Hypophosphite Hybrid Perovskite
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.0c01654
_journal_year                    2020
_chemical_formula_moiety         '0.11(H24 Mg4 O24 P12), 0.44(C H6 N3)'
_chemical_formula_sum            'C2 H24 Mg2 N6 O12 P6'
_chemical_formula_weight         558.71
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                105.6168(12)
_cell_angle_beta                 91.0614(13)
_cell_angle_gamma                118.4817(15)
_cell_formula_units_Z            2
_cell_length_a                   9.00382(15)
_cell_length_b                   9.06181(12)
_cell_length_c                   15.7050(2)
_cell_measurement_reflns_used    9453
_cell_measurement_temperature    360(2)
_cell_measurement_theta_max      73.5300
_cell_measurement_theta_min      5.6620
_cell_volume                     1068.26(3)
_computing_cell_refinement       'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      360(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.963
_diffrn_measurement_device_type  'XtaLAB AFC12 (RINC): Kappa single'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0265
_diffrn_reflns_av_unetI/netI     0.0238
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.963
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            10482
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.963
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         73.801
_diffrn_reflns_theta_min         5.666
_diffrn_source                   'fine-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    5.875
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.59817
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    1.737
_exptl_crystal_description       block
_exptl_crystal_F_000             576
_refine_diff_density_max         1.028
_refine_diff_density_min         -0.736
_refine_diff_density_rms         0.093
_refine_ls_extinction_coef       0.0157(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     305
_refine_ls_number_reflns         4176
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.029
_refine_ls_R_factor_all          0.0458
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0578P)^2^+2.1729P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1153
_refine_ls_wR_factor_ref         0.1155
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4151
_reflns_number_total             4176
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            exp_38_11_360_00.cif
_cod_data_source_block           exp_38_11_360_00
_cod_database_code               4003654
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              65841
_shelx_hkl_checksum              5675